Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

No Downloads

Total views

1,106

On SlideShare

0

From Embeds

0

Number of Embeds

2

Shares

0

Downloads

22

Comments

0

Likes

1

No embeds

No notes for slide

- 1. OPTI 222 Mechanical Design in Optical Engineering Stress – Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the strains and can only be determined by experiment. One of the simplest tests for determining mechanical properties of a material is the tensile test. In this test, a load is applied along the longitudinal axis of a circular test specimen. The applied load and the resulting elongation of the member are measured. 17
- 2. OPTI 222 Mechanical Design in Optical Engineering In many cases, the process is repeated with increased load until the desired load levels are reached or the specimen breaks. Load-deformation data obtained from tensile and/or compressive tests do not give a direct indication of the material behavior, because they depend on the specimen geometry. However, using the relationships we previously discussed, loads and deformations may be converted to stresses and strains. P δ σ = ε= A L σ = normal stress on a plane perpendicular to the longitudinal axis of the specimen P = applied load A = original cross sectional area ε = normal strain in the longitudinal direction δ = change in the specimen’s gage length L = original gage length The resulting stress-strain curve or diagram gives a direct indication of the material properties. Note: Stress-strain diagrams are typically based upon the original cross sectional area and the initial gage length, even though these quantities change continuously during the test. These changes have a negligible effect except during the final stages of the test. 2017-T451 Aluminum Alloy Load-deformation data Stress-strain data Engineering stress and engineering strain are computed using the original specimen dimensions. 18
- 3. OPTI 222 Mechanical Design in Optical Engineering Ductile Material Test Specimen True stress and true strain are based upon instantaneous values of cross sectional area and gage length. 19
- 4. OPTI 222 Mechanical Design in Optical Engineering As shown in the previous diagram, the initial portion of the stress-strain diagram for most materials used in engineering structures is a straight line. For the initial portion of the diagram, the stress σ is directly proportional to the strain ε. Therefore, for a specimen subjected to a uniaxial load, we can write σ = Eε This relationship is known as Hooke’s Law and was first recorded by Robert Hooke, an English mathematician, in 1678. Note: Hooke’s Law describes only the initial linear portion of the stress-strain curve for a bar subjected to uniaxial extension. The slope of the straight-line portion of the stress-strain diagram is called the Modulus of Elasticity or Young’s Modulus. E = σ/ε (normal stress – strain) G = τ/γ (shear stress – strain) E = Elastic Modulus or Modulus of Elasticity G = Shear Modulus or Modulus of Rigidity Material Properties σPL ⇒ Proportional Limit - Stress above which stress is not longer proportional to strain. σEL ⇒ Elastic Limit - The maximum stress that can be applied without resulting in permanent deformation when unloaded. σYP ⇒ Yield Point - Stress at which there are large increases in strain with little or no increase in stress. Among common structural materials, only steel exhibits this type of response. σYS ⇒ Yield Strength - The maximum stress that can be applied without exceeding a specified value of permanent strain (typically .2% = .002 in/in). 20
- 5. OPTI 222 Mechanical Design in Optical Engineering σU ⇒ Ultimate Strength - The maximum stress the material can withstand (based on the original area). Material Properties E ⇒ Modulus of Elasticity - Slope of the initial linear portion of the stress-strain diagram. The modulus of elasticity may also be characterized as the “stiffness” or ability of a material to resist deformation within the linear range. E (Steel) ≈ 30 x 106 psi E (Aluminum) ≈ 10 x 106 psi Et ⇒ Tangent Modulus - Slope of the stress-strain curve above the proportional limit. There is no single value for the tangent modulus; it varies with strain. G ⇒ Shear Modulus - Slope of the initial linear portion of the shear stress-strain diagram. G (Steel) ≈ 12 x 106 psi G (Aluminum) ≈ 4 x 106 psi Percent Elongation - The strain at fracture in tension, expressed as a percentage = ((final gage length – initial gage length)/ initial gage length) x 100. Percent elongation is a measure of ductility. Percent Reduction in Area - The reduction in cross-sectional area of a tensile specimen at fracture = ((initial area - final area)/ initial area) x 100. Percent reduction in area is also a measure of ductility. Isotropic – Isotropic materials have elastic properties that are independent of direction. Most common structural materials are isotropic. Anisotropic – Materials whose properties depend upon direction. An important class of anisotropic materials is fiber-reinforced composites. Homogeneous – A material is homogeneous if it has the same composition at every point in the body. A homogeneous material may or may not be isotropic. 21
- 6. OPTI 222 Mechanical Design in Optical Engineering Materials may be divided into two broad categories (ductile materials and brittle materials). Ductile Material – Materials that are capable of undergoing large strains (at normal temperature) before failure. An advantage of ductile materials is that visible distortions may occur if the loads before too large. Ductile materials are also capable of absorbing large amounts of energy prior to failure. Ductile materials include mild steel, aluminum and some of its alloys, copper, magnesium, nickel, brass, bronze and many others. Brittle Material – Materials that exhibit very little inelastic deformation. In other words, materials that fail in tension at relatively low values of strain are considered brittle. Brittle materials include concrete, stone, cast iron, glass and plaster. Failure Modes Brittle materials fail due to tensile (normal) stresses and rupture occurs along a surface perpendicular to the load. Ductile materials usually fail on planes that correspond to the maximum shear stresses (45°). A cup and cone failure is typical for ductile materials with the sides of cup and cone inclined at approximately 45° to the specimen axis. Poisson’s ratio – The ratio of lateral or transverse strain to the longitudinal strain. εt ν =− εa 22
- 7. OPTI 222 Mechanical Design in Optical Engineering εy ε ν =− =− z εx εx νσ x εy = εz = − E Poisson’s ratio for most materials ranges from 0.25 to 0.35. Cork ⇒ ν ≈ 0.0 Steel ⇒ ν = 0.27 – 0.30 Aluminum ⇒ ν = 0.23 Rubber ⇒ ν ≈0.5 (limiting value for Poisson’s ratio) Hot Rolled Steel COMPARISON CHART Est. Min Mechanical Properties – Based on ¾” – 1 ¼” RD. Bars Analysis Tensile Yield Elong. Red. Machin or Strength Strength in of Brinell -ability Trade Name psi psi 2” Area Hardness RatingH ASTM A36 ……………... 58,000 ….... 36,000 …. 23 … 21 ….. - …….. - M1010 47,000 26,000 28 50 95 - M1044 80,000 44,000 16 40 163 65 1080, 1020 ……………… 58,000 ….... 32,000 …. 25 … 50 … 116 ……..52 1035 72,000 39,500 18 40 143 65 1040 76,000 42,000 18 40 149 63 1045 82,000 45,000 16 40 163 56 Rycase (1117) ………….. 62,000 …...345,000 …. 23 … 47 …. 121 ……. 90 Leaded Rycase (11L17) 62,000 34,000 23 47 121 100 Rytense (1141) 94,000 51,500 15 35 187 65 Leaded Rytense (11L41) 94,000 51,500 15 35 187 95 Rytense 44 (1144)………. 97,000 …….53,000 …. 15 … 35 …. 197 ……. 64 HAiSi 1112 equals 100. 23

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment